Solid.Srorr Electronics Vol. 25. No. IO. pp. 10271031. 1982 Prmted in Great Britain.
W38I 1011821101027~)5$03.w/0 Pergamon Prers Ltd
NEW METHOD FOR THE DETERMINATION OF THE SURFACE BARRIER HEIGHTS IN MIS TUNNEL DIODES (SOLAR CELLS) S. K. KRAWCZYKt Institute of Electron Technology, Technical University of Warsaw, Koszykowa 75,00662 Warszawa, Poland (Received 15 July 1981;in revised form 23 February 1982) AbstractThe methods commonly applied for the determination of the surface barrier heights of Schottky diodes are usually extended for the MIS tunnel structures characterization, although, in such cases both, their range of application and accuracy are often strongly reduced. In this paper a new photoelectric method for the determination of the surface barrier heights in MIS tunnel diode is proposed together with experimental results supporting its validity. The presence of the ultrathin oxide layer between the metal and semiconductor does not reduce method’s applicability as long as the direct semiconductormetal tunneling is a dominant current flow mechanism through the oxide layer. In the contrary to the previous methods it allow us to measure directly the barrier height for minority carriers, and therefore, is especially recommended for minority carrier dievices. 1.
INTRODUCTION
The surface barrier heights in MIS tunnel diode (Fig. 1) can be considered as ones of the most important parameters of such structures. They influence directly the current flow mechanism in tunnel devices and the opencircuit voltage of MIS solar cells. Several methods for the barrier heights determination in metalsemiconductor contact have been worked out in the past [e.g. I]. The same methods are often applied for the case of metalinsulatorsemiconductor tunnel diodes [e.g. 2, 31, although it is well known, that in such structures they usually gives less accurate results. A common method for measuring the barrier heights of Schottky diodes is based on the plotting the inverse of the square of device capacitance as a function of the gate voltage [I, 4, 51. In MIS tunnel diodes, however, the application of this method can lead to less accurate results due to the presence of ultrathin insulating layer separating the metal and semiconductor, and in some cases also due to the formation of the inversion layer at the semiconductor surface[S71. The other method [e.g. I, 21, is based on the currentvoltage characteristics of Schottky diodes. In such case the barrier height for majority carriers can be calculated from the value of the extrapolated saturation current. Unfortunately, the tunneling through the oxide considerably reduces the current of the MIS tunnel diode as compared to the Schottky diode. In consequence, this method can be applied in the former case only when the exact values of the effective dielectric thickness and semiconductor to oxide affinity are known. Furthermore, the above procedure, as well as the other method involving the Richardson plot I/T2 vs l/nT [e.g. l31 can not be applied, for minority carrier devices, because minority carrier current is usually limited by generationrecom
binationdiffusion processes or tunneling[l, 91 and not by the thermonic emission. The direct measure of the surface barrier height can be also obtained from the threshold energy for photoexcitation of majority carriers into the semiconductor[l, IO]. However, this method again leads to inaccurate results since it does not take into account the effects of the barrier height lowering and photonassisted tunneling[ I l131. In this paper the new method for the barrier height determination in MIS tunnel structures is developed both, theoretically and experimentally. It is believed that the proposed method is more accurate than previously used ones. In contrast to other methods listed above presence of the ultrathin interfacial oxide do not reduce the accuracy of the method being proposed. Furthermore, the proposed method allow us to measure directly the barrier height for minority carrier devices such as some types of MIS solar cells. 2. THEORY In Fig. 2 the energy band diagram of the illuminated AlSiO,Si (ptype) tunnel diode is shown. Photoelectrical properties of such structure can be described by
M
1 S
EC

EF E”
E
Wurrently with Laboratolre d’Electronique,Automatiqueet Mesures Electriques, Ecole Centrale Collongue, 69130 Ecully, France.
de Lyon,
36 av. G. de
Fig. 1. Definitions of the barrier heights for minority & and majority EBp carriers in AlSi02Si (ptype) tunnel diode.
1027
1028
S.
K.
KRAWCZYK
I,< = IcTo[
[email protected],,
II
(8)
AU,, = AU,
(9)
Differentiating now eqn (7) and eqn (8) the following equations are obtained:
AL‘
=II,,,exp(AUJn)$F A&h Fig. 2. Energy band diagram of illuminated AlSO&ii (ptype) MIS tunnel diode. the set of following equations[8,
PI’ [exp(+)
_, ilr,,,, A&h
I
(IO)
9, 151:
(11) Z=
l,,h r,,,[exp(AUdn)llI,,[exp(
UG)11 (1)
Z,,,[exp(AU,)ll=Ip~Z~D~[exp(AU~n)
11
Equations (10) and (11) can be transformed to the single relation, which at Z,,. = 0 (when AU, = AU, = 0), can be simplified to the following form:
(2) Al,, U, =A&AU,
(3)
where Z is the total MIS current, Ioh is the current of light generated carriers, U, is the gate voltage in kT/q units, and where AUF = [E.+(O)  &,K9lIkT
(4a)
I
AZ,,, u,=o, I,, =o = , + Imw I I,.,,, n
(12)
If the generationrecombinationdiffusion current lRDO is dominated by recombination processes (typical case for MIS structures on silicon at temperatures lower than 35G370 K), then:
and
AU, = [&n(O)
 E,,I/kT.
(4b)
Currents ZCTO,ZVTo and lRDo in eqns (I, 2) stand for “zero currents” for electron tunneling, hole tunneling and generationrecombinationdiffusion processes, respectively. In general, currents lcTO, Zvro and lRDo depend on the gate voltage and illumination intensity. For the gate voltage equal zero and under the weak illumination the Zero, ZvTc)and I,,,, can be described as follows[l4, 16, 171: 1cTu = A,T’ exp (  x~“*xo) exp (  E,./kT)
(5)
1“TO  A, T2 exp ( x,,“~.x,,)exp ( E,,/kT)
(6)
where xc, xc = semiconductor to dielectric affinity for electrons and holes, respectively and A,, A,, = Richardson constant for electrons and holes, respectively. Furthermore, for zero gate voltage UC = 0, eqns (l)(3) can be reduced to the following form:
where q = electronic charge, ni = carrier concentration in intrinsic semiconductor, T. = electron carrier lifetime in a ptype semiconductor and xd = depletion region width. Assuming additionally, that in these conditions the value of n in eqn (2) do not depend on temperature,t then, on the basis of eqns (5) and (13) the following relation can be written:
2
 &
exp [(  EC;/2 f &,)/kTl
(14)
where EC is the energy band gap. Combining now eqn (12) and eqn (14) we obtain the following relation: I .Ur/AIp~ UC;=o, 17,=o 1T “’ exp [(  EC;/2+ E,,)/kT].
(l4a)
(7)
It is easy to notice, that by the determination of the ratio AZJAZ,, for Z,, = 0 at various temperatures, and by ploting:
tin fact, as temperature increases, the contribution of the diffusion current to the total I RW current also increases, which causes that the value of n decrease slightly. However, as long as recombination processes are much more efficient that diffusion processes, or when diffusion processes are much more efficient than recombination processes, this assumption is reasonable[ll].
the barrier height for minority carriers Es,, can be determined. Considering now the conditions, when diffusion processes are dominant, the current lRDo can
ZS, = Zph Ldexp
(AUJn)  11
New
be
written
method
for the determination
of the surface
in the following form: 2 0
(15)
 T exp [(I&
c
heights
Al 
T =
310 K
0.6
05
5%
1029 
Si
xo
24
A
9 
13 Qcm
tpl
2
where NA = concentration of acceptor ions per unit volume and D,, = electron diffusion coefficient. Assuming as previously, that in this conditions the value of n do not depend on temperature,t the following relation can be formulated: p
barrier
 E,,)/kT].
CT0
Combining eqn (12) and eqn (16) we obtain now the following relation: 1 Al,c/Alp,,
u,
=o, I,, =0
 I  T exp [  (&  E,.)/kTl.
16
(17) Consequently, by the determination of the value AZJAZ,, for I,, = 0 at various temperatures, and by ploting:
0.1
0.3
Q2
0.1
0
0.1
[VI
v,
Fig. 3. IV characteristicsof the MIS tunnel diode taken in dark at various temperatures. the barrier height for minority carriers Err. can be determined, under the conditions when the diffusion processes are more efficient than recombination processes. 3. SAMPLE PREPARATION
AND MEASURING
SETUP
In this study the MIS tunnel diodes were fabricated using (100) oriented, ptype, 2 fi cm singlecrystal silicon wafers. After the standard cleaning and etching procedure the ultrathin oxide (2030 8, thick) was grown on silicon by the d.c. plasma anodization[ltJ]. The oxide thickness was measured by the ellipsometry. As a gate, the semitransparent vacuum evaporated aluminium about 100A thick was used. A heavy Allayer was evaporated on the back side of the wafer to provide the ohmic contact. The completed devices were mounted in the test fixture where the measurements could be performed at any temperature between 300 and 450K with accuracy about 1 K. The illumination of A = 0.9 pm was provided by a CQYP 20 LED. 4. EXPERIMENTAL
the dark and under the illumination, respectively. Figure 5 shows the ZLD= IL  ZDas a function of gate voltage V,. When MIS tunnel diode is reversely biased with gate voltage V, s kT/q which results in AU, 4  1, the dark
2
AlSi02Si
lpi
x0 24 A z
L
‘0
9
13 Qcm
Ml
III//
6
” 1
6_
I1111
I lO1
RESULTS AND DISCUSSION
For the determination of the barrier height on the basis of eqn (14), it is necessary to determine the AZ,,/AZ,, ratio at various temperatures. The first step in our experimental procedure was to measure the sets of IV characteristics in the dark and under the illumination for several light intensities, at various temperaures. As an example, Fig. 3 and Fig. 4 show the sets of IV characteristics in the dark and under the illumination at various temperatures. In these figures ZDand I,_ stand for the current of the MIS diode in
vG [VI Fig. 4. IV characteristicsof the illuminated MIS tunnel diode taken at various temperatures.
1030
S.
K.
KRAWCZYK
is a consequence of the fact, that for the wavelength A = 0.9 pm the charge carriers are generated in the semiconductor quasineutral region rather than in the space charge region. As a result, the current Iph does not depend on the space charge region width and gate voltage. Measurements performed for several light intensities made it possible to notice that under experimental conditions applied in this study, the Zph was directly proportional to the light intensity, and that the ratio Z,,./Z,, was almost independent on the light intensity. These effects are due to low value of the light intensity in this experiment Under such conditions we have asumed, that:
2220
T 
310K
12+
y
lo
J
=
AlSi02St(p)
a
X0 6s
13
2AZ AZ,,
2L A Qcm
42
01
’
0.6
’
0.5
’
0.4
’
0.3 v,
’
42
’
0.1
’
0
u.1
[VI
Fig. 5. Plot of the difference between current of illuminated and nonilluminated MIS tunnel diode vs gate voltage at various temperatures.
current, as we can see from eqn (1) can be expressed by
Under the illumination and at the same gate voltage, the MIS current equals:
I,, =O, if,;=0
The determination of the Z,,/ZDhratio at various temperatures makes it possible now to evaluate the MIS barrier height by ploting In T”*(Z,,,/Z,,  I) vs I/T. Figure 6 illustrates such plot, and shows the band diagram of the semiconductor surface region resulting from this measuring procedure. As we can see from Fig. 6 in the examined device, the barrier height for minority carriers E HII, and for majority carriers E,,,, = EC; &,, equal 0.297 and 0.803 eV, respectively. For various devices from the same experimental run we have obtained the EBp values ranging from 0.787 to 0.819eV. In each case, these values were about 0.02 to 0.03 eV lower than the barrier heights calculated from the l/c’ vs V plot, and 0.01 to 0.02eV higher that those obtained from the Fowler plot. It is believed that the above differences are due to the effects discussed in the
first section of this work.
41s102
Thus, the value of I,,,, can be determined as a difference between IL and ZD currents for V, ti (kT/q). The procedure for the Z,,, determination is demonstrated in Fig. 5. We have observed the current of light generated carriers Z,,,,increases with increasing temperature. This is a consequence of the lifetime of minority carriers and absorption coefficient increase with the increase of temperature [ 19221. On the other hand, the Z,,/ZPhratio decreases considerably with increasing temperature. This in turn is due to the fact, that under the short circuit conditions,
a displacement
between
the quasiFermi
levels at the semiconductor surface occurs[23]. This displacement is as we can see from eqn (2) a driving force for the resultant minority carrier tunnel current. It also causes, that under the shortcircuit conditions the generationrecombinationdiffusion current ZRDO does not equals zero. As the temperature increases the ZRDo increase faster than Z,,, and the ZSC/ZP,, ratio decreases. In our experiments, the curves ZLDvs V, for V, ti
kT/q (Fig. 5) were usually so flat, that we had not difficulties with the determination of the lo,, value. This
_r, r,,,z
S(p)
1.L 1.21.o
0.8I0.6
\
,
EA
O.L
r 4% o.zMC( 4 =o S 0.2O.L
Bn

2.6
EA
0,297 ev 0.603 ev
E0p'
1
2.5
0,253 eV
EG/2'
EB"' E

I
2.7
I
I
,
I
1
1
2.6
2.9
3.0
3,l
3.2
3.3
VT
:I.4
[xIO~ K‘1
Fig. 6. The proposed procedure of the barrier height determination.
New methodfor the determinationof the surface barrier heights Considering the error of the proposed method, it appears that the error may arise from the presence of series resistance R, of the MIS tunnel device. However, simple evaluation shows that for low values of Zph and I,, currents, this effect should be negligibly small. In typical MIS solar cells, as well as in our samples the value of R, do not exceed few ohms. Even for the series resistance as high as R, = lOOR the voltage drop across R, is lO‘V and remains lower than kT/q. Another possible error of the proposed method is due to the neglecting of the diffusion or recombination processes, as well as the assumption that the value of n do not depend on temperature. This error, however, can be minimalized by choosing an appropriate range of temperature, and by proper interpretation of the measurement results, accordingly to eqn (14) or eqn (16). Since eqns (5) and (6) are based on the assumption, that direct semiconductormetal or metalsemiconductor tunneling is a dominant currentflow mechanism through the insulating layer, the proposed method may to some extend be restricted in structures with oxide thicker than about 50 A. On the other hand, for oxide thickness of the order of a few angstroms, the I<, may be very close to Zp,,, and ‘it may be difficult to notice the difference between them. 5. CONCLUSIONS In this work a new method for the determination of the barrier height in MIS tunnel diode has been proposed together with the experimental results supporting its validity. Proposed method allow us to measure directly the barrier height for minority carriers, and therefore it seems to be especially useful for minority carrier MIS tunnel diodes. Presence of ultrathin oxide do not reduce method accuracy as long as the direct semiconductormetal tunneling is a dominant current flow mechanism trough the oxide layer.
1031
Acknow/edgementI
wish to thank Professor P. Viktorovitch for critical reading of the manuscript and helpful suggestions.
REFERENCES
1. E. H. Rhoderick, MetalSemiconductor Contacts. Clarendon Press, Oxford (1978). 2. E. J. Charlson and J. C. Lien, J. Appl. Phys. 46, 3982(1975). 3. S. Ashok, J. M. Borrego and R. J. Gutmann, SolidSr. Electron. 22, 621 (1979). 4. A. M. Cowley, 1. Appl. Phys. 37, 3024(1%6). 5. A. M. Goodman, L Appl. Phys. 34,329 (1963). 6. R. F. Schwarz and J. F. Walsh, Proc. IRE 41, 1715(1953). 7. M. A. Green, SolidSt. Electron. 19,421 (1976). 8. J. Shewchun. R. Sinah and M. A. Green. J. Aool. . . Phvs. _ 48. 765 (1977). 9. K. K. Ng and H. C. Card, IEEE Trans. Electron. Deu. ED27, 717 (1980). IO. R. H. Fowler, Phys. Rev. 38, 45 (1931). 11. R. J. Archer and T. 0. Yep. J. Appl. Phys. 41, 303 (1970). 12. C. R. Crowell, T. W. Kao, C. L. Anderson and V. L. Rideout, Surface Sci. 32, 591 (1972). 13. C. L. Anderson, C. R. Croweli, T. W. Kao, SolidSt. Electron. 18, 705 (1975). 14. H. C. Card, SolidSr. Electron. 20, 971 (1977). 15. S. K. Krawczyk, Proc. Internal. Conf. Insul. Films on Semicond. INFOS 81, Erlangen, 2729 April (1981). 16. G. P. Srivastava, P. K. Bhatnagar and S. R. Dhariwal, SolidSt. Electron. 22, 581 (1979). 17. S. K. Krawczyk, Physica Status Solidi (a), 69, K77 (1982). 18. R. B. Beck, A. Jakubowski and J. RuzyYYo.Proc. Inf. Con/. Insul. Fihns on Semicond. INFOS 81, Erlangen, 2729 April (1981). 19. H. J. Hovel, Semiconducfor and Semimetales, Vol. II, Solar Cells. Academic Press, New York (1975). 20. A. Agarawalla, V. K. Tewary, S. K. Agarwal and S. C. Jain, SolidSt. Electron. 23, 1021(1980). 21. D. W. Spaderna and H. Navon, Trans. Electron. ED25, 1290 22. K. R. Singh J. Shewchun, Electron. 22,793 23. S. Krawczyk, A. Celk, 187(1981).
and M.
Solar